Wood properties of detarium senegalense, a lesser used tropical timber growing in nigeria.
Journal of Biology, Agriculture and Healthcare www.iiste.orgISSN 2224-3208 (Paper) ISSN 2225-093X (Online)Vol 2, No.10, 2012 Wood Properties of Detarium senegalense, a lesser used tropical timber growing in Nigeria. Ogunwusi, Abimbola Raw Materials Research and Development Council, Abuja firstname.lastname@example.orgAbstractThe wood products sector in Nigeria is currently performing below optimal capacity as a result of increasing scarcityof economic wood species. In order to adequately cater for products requirement of Nigerians locally, the sector hasincorporated lesser used wood species into its stream of raw materials requirement. One of these species commonlyfound in sawmills and plank depots in the country is Detarium senegalense. As the properties of wood determine itsutilization potentials, this study was carried out to determine the wood properties of D. senegalense. The basicdensity is 610kg/m3. This is within the range of the economic species currently used in the wood products sector.However, the heartwood constitutes only 9.02% of the total volume fraction. The sapwood constitutes 75.98%, andthe bark 15%. The low percentage of heartwood in contrast with the high volume of sapwood indicated that thewood may not be durable in service. The mean age is 47 years while the mean diameter is 21cm indicating that it isa small diameter hardwood. The vessels elements, fibres, axial and ray parenchyma cells constitute 9.28, 31.4, 30.6and 28.72% respectively. The number of vessel per mm3 is 13.62 while those of fibres are 3301 per mm3. Therelative high proportions of the fibres may have contributed to its high density.1.0 IntroductionThe wood and wood products sector of the national economy is currently facing wood shortage problems.According to RMRDC (2010) the total volume of useable wood down to 30cm cutting diameter in the reserved forestareas is 239,775,500 m3. This by comparison is not significantly different from 473, 509,205.943 m3 reported byAkindele et al (2001). Considering the ten years difference between the reporting periods, when there figures arejuxtaposed with total wood requirement projected at 59,955, room per 2010 (FMAWRRD, 1988; Bourgione,1991),extreme wood shortages are expected within the next 10-15 years. Many of the forest reserves are presentlydepleted to such a level that the traditional valuable economic large–size logs are becoming increasingly difficult tocome by.In order to adequately meet the demand for wood products, some new indigenous woods are being introduced intothe timber market as substitutes to those traditional economic hardwoods that are fast disappearing. Detariumsenegalense is one of the lesser-known tree species that is presently finding its way to our timber market as apotential valuable wood for various end uses. These lesser used timber were once neglected in the forest reserves infavour of the economic tree species, which were then readily available.A survey of available literature revealed the paucity of documented information on the wood properties of theDetarium senegalese. In particular, no information could be found on its anatomical properties vis-à-vis its woodcellular composition. As a biological material, the properties of wood determine its industrial application. Ittherefore becomes imperative that a thorough knowledge of its anatomical properties should precede the selection orchoice of the wood species for end use. The present study was embarked upon in this regard, to evaluate thecellular the wood properties of the plant species. Emphasis is placed on the wood density, fiber characteristics andwood cellular structure to ascertain its usefulness in the wood products sector of the national economy.2.0 Materials and Methods 100
Journal of Biology, Agriculture and Healthcare www.iiste.orgISSN 2224-3208 (Paper) ISSN 2225-093X (Online)Vol 2, No.10, 20122.1 Field SamplingThe materials used for the study were obtained from the natural forest in the savanna area Okeawon, near Jebba inKwara State (Latitude 9.300N. Longitude 4.460E.The sampling procedure employed by Onilude et al (1988) was used for the study. The sampled trees were selectedat random, felled, sample discs about 7.5cm thick were taken at the breast height. The sampled discs wereimmediately wrapped in plastic bags to prevent loss of moisture during transportation.2.2. Laboratory procedure2.2.1 Determination of Wood Microscopic ConstituentsLaboratory study was carried out on the entire discs to determine the tree age and volume fractions of heartwood,sapwood and bark of the discs. Tree age was determined using sand paper to brush the discs and a hand lens wasused to count the rings. The grid point method using a 120-point circular grid (Ifju, 1981, Onilude et al, 1988,Ogunwusi, 1991), was employed for the determination of volume fractions of heartwood, sapwood and bark of thewood. After this, the sampled discs were debarked for other subsequent analysis.From the debarked discs, strips 5cm wide were removed and each strip was further sawn in half through the pith.One half was used for fibre length and density determination, while the other was employed for alcohol benzenesoluble extractable content tests.2.2.2 Basic Density DeterminationTest blocks for density determination were partitioned into three zones representing the heartwood (taken at fourrings from the pitch) transition wood (between heartwood and sapwood zones) and the sapwood zones (taken at fourrings from the bark).The basic density of samples was obtained as the oven weight (103+ 20C) to green volume ratios.2.2.3 Fibre Length DeterminationSamples for fibre length determination were obtained as thin slivers taken from sides of the wood blocks used fordensity determination. The samples were macerated in 1:1 solution of glacial acetic acid and hydrogen peroxide asdescribed by Franklin (1946). The mixture was autoclaved at constant temperature and pressure of 120 0C and1.00kgf/cm2 for 45 minutes. The macerated samples were later rinsed thoroughly in water and a total of 15projected whole fibre images measured from each sampling zone.2.2.4 Alcohol/Benzene Solubility DeterminationExtractive contents of sampled trees were determined on the entire second half of the diameter strip. Samples usedfor extraction were debarked and prepared in accordance with ASTM Standard - D1107 – Standard Method forAlcohol/Benzene Solubility of Wood. At the end of each successive extraction process, the samples were oven driedto constant weight. The extractive contents were then determined based upon initial oven dry mass.3. Results and discussionTable 1 present the results of the wood properties evaluation. The density decreased from 640kg/m3 in the heartwoodto 635km3 in the transition wood and to 556 kg/m3 in the sapwood zone. Radial decrease in density from the pith tothe bark as exhibited by this species has been reported in Butyrospermum paradoxium and Albizia zygia byOgunwusi (1991) and in Prospsis africana by Onilude et al. (1988). The mean basic density is 610 kg/m3. This iswithin the range of reported for economic wood species that are currently utilized in the wood and wood productsindustry. For instance the wood density of Terminalia superba is reported as 465kg/m3, Terminalia ivorensis,576kg/m , Mansonia altissima,672kg/m3 and Tectona grandis 640kg/m3 (Aribisala,1993). On density basis, the 3 101
Journal of Biology, Agriculture and Healthcare www.iiste.orgISSN 2224-3208 (Paper) ISSN 2225-093X (Online)Vol 2, No.10, 2012wood can be used where the aforementioned commercial species are deployed.The fibre length increased from 0.95 mm in the heartwood to 0.96 in the transition wood, and then increased to 1.19mm in the sapwood zone. The mean fibre length is 0.91 mm. This is within the range of fibre lengths of mosthardwood species, indicating, that apart from its use in the wood industry, the plant species can also be used as asource of short fibre raw material in the nation’s pulp and paper sector (Ogunwusi,1991). The alcohol benzenesoluble extractive content of the wood species ranged from 2.60-2.70% with a mean of 2.67 %. This is within therange of 2 to 4 % reported as suitable for pulp and paper production in hardwood (Panshin and Zeeuw, 1980). Aswood extractives are the major cases of pitch deposition in pulp and paper mills, the higher the extractive content ofhardwoods, the greater the pitch deposition potentials during pulping (Allen,1988).The mean volume functions of heartwood, sapwood and bark of the tree species are also presented in Table 1.Heartwood constitutes only 9.02% of the total volume fraction; the sapwood, 75.98%, and the bark, 15%. The lowpercentage volume of heartwood in contrast to the high volume of sapwood indicated that the wood may not bedurable in service. The lifespan may be shorter than those of species with higher volumes of heartwoodpercentages. Heartwoods contain dead cells with deposited wood extractives which are toxic to wood destroyingagents such as insects and fungi attacks. Sapwoods on the other hand contain fluid that are easily attacked by wooddestroying agent (Ogbogu,1990). As a result, sustainable utilization of Detarium senegalense in the wood industrywill require pressure treatment to prolong the lifespan of the wood in service. The age range of the wood speciesutilized in this study varied from 29-67 years (Table 1). The mean age is 49 years. When this is juxtaposed withthe mean diameter of 21cm and a diameter range from 14.3cm to 27.0cm, it showed that the wood species is a smalldiameter wood species. More recently, it has recommended that saw millers and other practitioners in the nation’swood industry re-strategize to handle small diameter wood species. This is imperative as the large diameter woodspecies have become scarce in the nation’s forest reserves (RMRDC, 2010).Table 2 shows the result of the quantitative characterization of the wood elements of the plant species. The presenceof vessels in hardwood differentiates them from softwoods. The proportion and distribution of anatomical elementsare of importance in determining the structural characteristics and quality of wood for a particular purpose.Increase in the proportion of vessel elements may lead to decrease in wood density and an increase in the number ofweak points along the surface of the wood. These may serve as pathway for bacteria, fungi and virus infections inthe wood leading to increase in wood deterioration (Akachukwu,1979). Vessel elements, fibres, axial and rayparenchyma tissues constitute 9.2, 31.4, 30.6 and 28.72% of the volume fractions of the wood elements respectively.The number of vessels per mm2 of wood is 13.62 while those of fibre are 3301 per mm3. The relative proportions offibres play an important role in the determination of wood for various end uses. The high proportion of fibres maybe responsible for the high density of the wood species.4. ConclusionThe decreasing availability of preferred wood species in the nation’s forests have necessitated introduction of newwood species into the mainstream of raw materials utilized in the wood product industries. This development hashowever led to production of lesser quality products. While substitution or complementary utilization of lesserutilized wood species has become a necessity, it is imperative that any material to be sued as substitutes should atleast possess minimum criteria that will make it durable when deployed in the industry. From the findings of thisstudy, Detarium senegalense is a good substitute to traditional raw materials use in the sawmill and furnitureindustries due to its density. However the high proportion of sapwood it contains necessitated that adequatepreservative treatment is applied before its deployment for service to increase its lifespan. The presence of vesselsand parenchyma’s cells will assist in promoting wood preservatives penetration into the wood during treatment.ReferenceAkachukwu, A.E (1979): Variation in wood anatomy of Angiosperms (Hardwoods) as a guide to forest management.Univ. of Ibadan Agric. Bulletin., 2(1):1-26 102
Journal of Biology, Agriculture and Healthcare www.iiste.orgISSN 2224-3208 (Paper) ISSN 2225-093X (Online)Vol 2, No.10, 2012Akindele, S.O, Dyck.J.,Akindunmi, F.F,Papka, P.M, and Olaleye, O.A. (2001) Estimate of Nigeria`s TimberResources. In L Popoola, J.E. Abu and P.I Oni ed. Proceedings of the 27th Annual Conference of the ForestryAssociation of Nigeria, Abuja FCT. Pp1-11Allen, L.H. (1988): Pitch Control: Optimisation of Alum usage in Newsprint Mills. Pupl and Paper Can 89(10)T342-346.American Standard Testing Methods (2007) D1107- Standard Method for Alcohol Benzene Solubility of WoodAribisala, O.A. (1993): Raw Materials Revolution and Impact on Industrialisation in Nigeria. Mednet PublicationsLtd. (1993). ISBN 978 – 024 – 000 – 4.Bourgione, J. (1991): Demand and Supply of Forestry Products in Nigeria. World Bank.Washington D.C.FMAWRRDC (1988): Perspective Plan for Agricultural Development in Nigeria. Policies and Programmes forForestry and Wildlife Development.Franklin, G.L. (1946): A rapid method of softening wood for microtome sectioning of tropical woods. Oxford Univ.Press. Ltd, London. 19. 195Ifju, G. (1983). Quantitative wood anatomy- Ceratain Geometrical-Statistical Relationships. Wood Fibre Sci., 15(4);326-334.Ogbogu, G.U (1990): Problems Associated with the use of wood in Building construction in Nigeria and possiblesolutions. In Gob Dada and P.C. Obiaga (Eds). Proceedings of the 20thAnnual Conference of the ForestryAssociation of Nigeria. Katsina, Katsina State pp 153-156Ogunwusi, A.A. (1991): The Influence of wood quality and pulping variables on pitch deposits and on properties offifteen Nigerian Hardwoods. Ph.D Thesis. Faculty of Technology, University of Ibadan. Unpublished.Onilude, M.A, Dada, S.A and Ogunwusi, A.A. (1988): Wood Properties of Five Selected Nigerian Trees Growing Inthe Savanna Belt. Nig. Jour. For. 18(1 and 2): 3-8.Panshin, .J and DeZeew, C. (1980): Textbook of Wood Technology. McGraw Hill Bk. CoyRMRDC (2010) Report on the Multi Disciplinary Task Force on Wood and Wood Products Sector RMRDC.Unpublished. RMRDC (2010): Report of the Multidisciplinary Task Force On Wood and Wood Products. Raw MaterialsResearch and Development Council Publication. 103
Journal of Biology, Agriculture and Healthcare www.iiste.orgISSN 2224-3208 (Paper) ISSN 2225-093X (Online)Vol 2, No.10, 2012Table 2: Mean and Standard deviation of point count for cell types of Detarium senegalense*Each value was calculated from a total of 4 stereological 105
This academic article was published by The International Institute for Science,Technology and Education (IISTE). The IISTE is a pioneer in the Open AccessPublishing service based in the U.S. and Europe. The aim of the institute isAccelerating Global Knowledge Sharing.More information about the publisher can be found in the IISTE’s homepage:http://www.iiste.org CALL FOR PAPERSThe IISTE is currently hosting more than 30 peer-reviewed academic journals andcollaborating with academic institutions around the world. There’s no deadline forsubmission. Prospective authors of IISTE journals can find the submissioninstruction on the following page: http://www.iiste.org/Journals/The IISTE editorial team promises to the review and publish all the qualifiedsubmissions in a fast manner. All the journals articles are available online to thereaders all over the world without financial, legal, or technical barriers other thanthose inseparable from gaining access to the internet itself. Printed version of thejournals is also available upon request of readers and authors.IISTE Knowledge Sharing PartnersEBSCO, Index Copernicus, Ulrichs Periodicals Directory, JournalTOCS, PKP OpenArchives Harvester, Bielefeld Academic Search Engine, ElektronischeZeitschriftenbibliothek EZB, Open J-Gate, OCLC WorldCat, Universe DigtialLibrary , NewJour, Google Scholar